Syntheses, Structure, and Bonding of Rb14(Mg1-xInx)30. A Nonstoichiometric Phase with an Unusual Substitution in the Anion Framework
Li, Bin; Corbett, John D.; Inorganic Chemistry 45 (2006) 156–161; doi:10.1021/ic0514290

data_4331698
_publ_section_title
;
 Syntheses, Structure, and Bonding of Rb14(Mg1-xInx)30. A
 Nonstoichiometric Phase with an Unusual Substitution in the Anion
 Framework
;
_journal_issue                   1
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              156
_journal_page_last               161
_journal_paper_doi               10.1021/ic0514290
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'In23.73 Mg6.27 Rb14'
_chemical_formula_weight         4073.68
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           189
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   10.0652(14)
_cell_length_b                   10.0652(14)
_cell_length_c                   17.947(4)
_cell_measurement_temperature    293(2)
_cell_volume                     1574.6(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'STOE IPDS'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0151
_diffrn_reflns_av_sigmaI/netI    0.0223
_diffrn_reflns_limit_h_max       0
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            1477
_diffrn_reflns_theta_full        29.23
_diffrn_reflns_theta_max         29.23
_diffrn_reflns_theta_min         2.27
_exptl_absorpt_coefficient_mu    19.308
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   X-shape
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.296
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1756
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.15
_refine_diff_density_max         1.574
_refine_diff_density_min         -1.056
_refine_diff_density_rms         0.219
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.0(4)
_refine_ls_extinction_coef       0.00069(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.963
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     51
_refine_ls_number_reflns         923
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.963
_refine_ls_R_factor_all          0.0334
_refine_ls_R_factor_gt           0.0282
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0098P)^2^+23.4956P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0537
_refine_ls_wR_factor_ref         0.0551
_reflns_number_gt                849
_reflns_number_total             923
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0514290sup1.cif
_cod_data_source_block           3"Rb14(Mg1-xInx)30,x=0.792"
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        1574.6(4)
_cod_original_sg_symbol_H-M      P-62m
_cod_database_code               4331698